those of HKUST-1, are immune to unwanted reduction by benzaldehyde. The Lewis-acid-catalyzed cyanosilylation of aromatic aldehydes has also been carried out by Long and co-workers using a MOF of the formula Mn3[(Mn4Cl)3BTT8(CH3OH)10]. This material contains a three-dimensional pore structure, with the pore diameter equaling 10 Å. In principle, either of the two types of Mn(II) sites could function as a catalyst. Noteworthy features of this catalyst are high conversion yields (for small substrates) and good substrate-size-selectivity, consistent with channellocalized catalysis. Encapsulated catalysts The MOF encapsulation approach invites comparison to earlier studies of oxidative catalysis by zeolite-encapsulated Fe(porphyrin) as well as Mn(porphyrin) systems. The zeolite studies generally employed iodosylbenzene (PhIO), rather than TPHP as oxidant. The difference is likely mechanistically significant, thus complicating comparisons. Briefly, PhIO is a single oxygen atom donor, while TBHP is capable of more complex behavior. In addition, for the MOF-based system, it is conceivable that oxidation proceeds via both oxygen transfer from a manganese oxo intermediate as well as a manganese-initiated radical chain reaction pathway. Regardless of mechanism, the approach is a promising one for isolating and thereby stabilizing the porphyrins against both oxo-bridged dimer formation and oxidative degradation. Metal-free organic cavity modifiers Most examples of MOF-based catalysis make use of metal ions or atoms as active sites. Among the few exceptions are two nickel- and two copper-containing MOFs synthesized by Rosseinsky and co-workers. These compounds employ amino acids(L- or D-aspartate) together with dipyridyls as struts. The coordination chemistry is such that the amine group of the aspartate cannot be protonated by added HCl, but one of the aspartate carboxylates can. Thus, the framework-incorporated amino acid can exist in a form that is not accessible for the free amino acid. While the nickel-based compounds are marginally porous, on account of tiny channel dimensions, the copper versions are clearly porous. The Rosseinsky group showed that the carboxylic acids behave as Brønsted acidic catalysts, facilitating (in the copper cases) the ring-opening methanolysis of a small, cavityaccessible epoxide at up to 65% yield. Superior homogeneous catalysts exist however. Kitagawa and co-workers have reported the synthesis of a catalytic MOF having the formula [Cd(4-BTAPA)2(NO3)2]. The MOF is three-dimensional, consisting of an identical catenated pair of networks, yet still featuring pores of molecular dimensions. The nodes consist of single cadmium ions, octahedrally ligated by pyridyl nitrogens. From a catalysis standpoint, however, the most interesting feature of this material is the presence